Home >Engineering >Concrete design mix (ss)

# Concrete design mix (ss)

Date post:08-Jan-2017
Category:
View:7,179 times
Transcript:
• 1

Concrete Mix Design

By K.Shah B.E.(Civil Engg) NIT Rourkela,India

M.Sc. (Environment), University of Leeds, UK

Ex-GM(Civil & Environment) MNC

Currently Guest faculty-College of Technology &

Engineering

• 2

Concrete Mix Design

Mix design is defined as the process of

selecting suitable ingredients of concrete

and determine their relative proportions

with the object of producing concrete of

certain minimum strength and durability as

economically as possible.

• 3

Variables in Proportioning :4 varaible

factors to be considered:

1. Water cement Ratio

2. Cement aggregate ratio

4. Consistency

• 4

In design mix ,generally 2-3 factors are specified

To use minimum amount of cement paste that

can lubricate the mass and will bind the

aggregates together and fill the space between

them.

Excess paste involves more cost, shrinkage,

impermeability etc.

Good gradation of aggregates to minimize voids.

• 5

Methods of Proportioning

1. Indian Standards Recommended method IS 10262-82

2. American Concrete Institute Method of Mix Design (ACI 211)

3. DOE method

4. Mix design for pumpable concrete

5. Indian Road Congress , IRC 44 method

7. Mix design based on flexural strength

8. Arbitrary proportion

9. Fineness modulus methods

10. Maximum density method

11. Surface area method

• 6

American Concrete Institute

Method of Mix Design (ACI)

Data to be collected:

a) Fineness modulus of fine aggregates

b) Sp gravity of coarse & fine aggregates

c) Absorption characteristics of coarse &

fine aggregates

d) Sp gravity of cement

• 7

STEPS IN ACI METHOD

1. From minimum strength specified, estimate average design

strength using standard deviation method

2. Find w/c ratio from table 2. Find water cement ratio for durability

from table 3. adopt lower value.

3. Decide maximum size of aggregate (generally 20 mm for RCC)

4. Decide workability in terms of slump for the type of job in hand.

Table 4.

5. Total water in kg/m3 is read from table 5 entering the table with

selected slump & selected maximum size of aggregate.

6. Cement content is computed by dividing total water content by w/c

ratio.

• 8

7. From table 4 the bulk volume of dry rodded coarse aggregate / unit

volume of concrete is selected, for particular maximum size of

coarse aggregate & fineness modulus of fine aggregate.

8. The weight of CA /M3 of concrete is calculated by multiplying the

bulk volume with bulk density.

9. The solid volume of coarse aggregate in one M3 of concrete is

calculated by knowing the sp. Gravity of CA

10. Solid volume of cement, water & volume of air is calculated in one

m3 of concrete

11. Solid volume of sand is calculated by substracting soild volume of

cement, CA,water, & air from total volume of concrete.

12. Weight of fine aggregate is calculated by multiplying the solid

volume of fine aggregate by sp gr of FA.

• 9

(1) Dry Bulk Volume of coarse aggregate/ unit volume of concrete as per ACI 211.1-91

Maximum

size of

aggregate

Bulk volume of dry rodded CA /unit volume of concrete for

fineness modulus of sand of

FM 2.4 2.6 2.8 3.OO

10 0.5 0.48 0.46 0.44

12.5, 0.59 0.57 0.55 0.53

20

(25,40,50,70)

0.66 0.64 0.62 0.60

150 .87 0.85 0.83 0.81

• 10

(2) Relation between water/cement ratio & average

compressive strength of concrete, as per ACI211.1-91

Average compressive

strength at 28 days

Effective water/cement ratio (by mass)

MPa Non air entrained

concrete

Air entrained concrete

45 0.38 -

40 0.43 -

35 (30,25,20) 0.48 0.4

15 0.8 0.71

• 11

(3) Requirements of ACI-318-89 for w/c ratio &

strength for special exposure conditions

Exposure condition Maximum w/c ratio,

normal density

aggregate concrete

Minimum design

strength, low density

aggregate concrete

MPa

Concrete intended to be

watertight

(a) Exposed to fresh water

(b) Exposed to sea water

0.5

0.45

25

30

Concrete exposed to

freezing in a moist condition

0.45 30

For corrosion protection of

reinforced concrete exposed

to de icing salts, sea water

0.4 33

• 12

(4) Recommended value of slump for various

types of construction as per ACI 211.1-91

Type of construction Range of slump (mm)

Reinforces foundation walls & footings 20-80

Plain footings,substructure wall 20-80

Beams & reinforced walls 20-100

Building columns 20-100

Pavements & slabs 20-80

Mass concrete 20-80

• 13

(5) Approximate requirements for mixing water & air content for

different workabilities & nominal maximum size of aggregates as per

ACI211.1-91

Non air entrained concrete

Workability

or air

content

(Slump)

Water content, kg/m3 of concrete for indicted maximum

aggregate size

10 mm 12.5 mm 20 mm 150 mm

( 25, 40,50,70)

30 -50 mm 205 200 185 125

80-100 mm 225 215 200 140

150-180 mm 240 230 210 -

Approx

entrapped

air (%)

3 2.5 2 0.2

• 14

(6) First estimate of density of fresh concrete as

per ACI 211.1-91

Maximum size of

aggregate (mm)

First estimate of density of fresh concrete

Non air entrained kg/m3 Air entrained kg/m3

10 2285 2190

12.5 (20,25,40,50) 2315 2235

20 2355 2280

150 2505 2435

• 15

(7) Required increase in strength (mean strength) for

specified design strength when no tests records are

available as per ACI 318-89

Specified design

strength (MPa)

Required increase in

strength (MPa)

Less than 21 7

21-35 8.5

35 or more 10

• 16

Example ACI method

Design a concrete mix for construction of elevated water tank.

a) Specified design strength = 30 MPa

b) Standard deviation = 4 MPa

c) Sp gr. FA & CA = 2.65 & 2.7

d) Dry rodded bulk density of CA = 1600 kg/m3

e) FM of FA = 2.8

f) Slump = 50 mm

g) CA is absorptive up to = 1 %

h) Free surface moisture in sand = 2 %

• 17

Calculation

Mean Strength fm = fmin+ks (k =1.64)

fm = 30+1.64x4 = 36.56 say 36.5

From table 2 w/c = 0.47

From exposure condition w/c = .5

Minimum of 0.47 & 0.5 = 0.47

From table 5 for slump 50 mm, 20 mm maximum aggregate & non air

entrained condition Mixing water is 185 kg/m3

Required cement content = 185/0.47 = 394 kg/m3

From table 1, for 20 mm CA, FA 2.8, the dry rodded bulk vol of CA = 0.62

Weight of CA = 0.62x1600 = 992 kg/m3

From table 6,the first estimate of density of fresh concrete for 20 mm CA &

non air entrained concrete is 2355 kg/m3

• 18

Weight of all ingredient :

Weight of water = 185 kg/m3

Weight of cement =394 kg/m3

Weight of CA = 992 kg/m3

Weight of sand = 2355 (185+394+992) = 784 kg/m3

• 19

ingredients Weight kg/m3 Absolute volume cm3

cement 394 394/3.15x103 = 125x 103

Water 185 185/1 x103 = 185x 103

CA 992 992/2.7 x103 = 367 x 103

air 2/100 x103 = 20 x 103

Total abs vol 697 x 103 cm3

• 20

Therefore absolute vol of FA =(1000 -697) X 103 = 303 103 cm3

Weight of FA = 303 x 2.65 = 803 kg/m3

Estimated qty of ingredients;

a) Weight of water = 185 kg/m3

b) Weight of cement =394 kg/m3

c) Weight of CA = 992 kg/m3

d) Weight of sand = 803 kg/m3

Proportion

C : FA : CA ; WATER

394: 803 : 992 : 185

1 : 2.04 : 2.52 : 0.47

For one bag of cement 50 kg Ratio in kg is = 50:102:126:23.5

• 21

Indian Standard Method of

Concrete Mix-IS 10262-1982

STEPS

• 22

IS Method - Step 1

Target mean strength of concrete

fck =fck1+tS

Refer table 1 & 2 for t & S

fck = strength at 28 days

fck1 = characteristics strength at 28 days

t = 1.65 = statistical value; (depends on

expected proportion of low results( risk factor)

S = standard deviation

• 23

IS Method Step 2

Selection of water cement ratio:

From graph 1 ,w/c ration corresponding to

target strength is determined.

• 24

IS Method Step 3

If 28 days strength of cement is known

then w/c ratio can also be calculated from

graph 2.

• 25

IS Method Step 4

Estimation of entrapped air:

Air content is estimated from table 3 for

maximum size of CA 